CATALYSTS AND ELECTRODES FOR THE ELECTROREDUCTION OF CARBON DIOXIDE TO USEFUL CHEMICALS
BY SICHAO MA
Submitted in partial fulfillment of the requirements for the degree of Doctor of Philosophy in Chemistry
in the Graduate College of the
University of Illinois at Urbana-Champaign, 2016
Urbana, Illinois Doctoral Committee:
Professor Paul J.A. Kenis, Chair Professor Andrew A. Gewirth Professor Catherine J. Murphy
Industrialization and increasing population have brought the world two major challenges: climate change and increasing energy demands. First, the atmospheric CO2 level has increased to
400 ppm, and already this high level has been associated with undesirable climate effects such as global warming and an increased occurrence of erratic weather. Second, the world faces challenges in meeting its energy needs due to increasing global population as well as the dwindling resources of fossil fuels on the earth. Various strategies such as switching from fossil fuel derived energy to nuclear energy or renewable energy sources (solar, wind, hydro) need to be pursued to curb the increase in atmospheric CO2 levels while decreasing our dependence on fossil fuels.
However, due to the lack of efficient ways for large-scale energy storage, significant amounts of renewable energy will be wasted when the supply is higher than the actual demand due to its intermittency. A potential strategy that can be employed to help overcome both challenges is the electroreduction of CO2 into useful feedstock chemicals or fuels such as formic acid, carbon
monoxide, hydrocarbons, and alcohols using otherwise wasted large amounts of intermittent excess renewable energy.
Although the electroreduction of CO2 offers the potential to recycle CO2 and store
intermittent renewable energy, this process is still not economically viable due to insufficient performance levels, specifically due to high overpotentials which reduce energy efficiency, low current densities and low selectivities. Better catalysts that show high activity as well as electrodes that exhibit excellent mass transfer capabilities and electron conductivities are needed. This dissertation reports the development of active and durable catalysts that exhibit low overpotentials
for the electroreduction of CO2 to products such as CO, C2H4 and/or C2H5OH. This dissertation
will also discuss the roles electrolytes and electrode structures play in the electroreduction of CO2.
The focus of Chapters 2 and 3 is on developing better cathode and anode catalysts for the electroreduction of CO2 to CO. Chapter 2 reports on the role of support materials on cathode
performance. Ag supported on TiO2 exhibited a twofold higher partial current density for CO than
Ag supported on C with the same Ag loading and similar performance compared to unsupported Ag nanoparticles, but at a 2.5 times lower Ag loading. The TiO2 support material was also found
to stabilize a reaction intermediate and serves as a redox electron carrier to assist the CO2 reduction
reaction. Chapter 3 reports how two forms of IrO2, dihydrate and non-hydrate, improve system
energy efficiency and production rate when used as the anode catalyst. For example, when IrO2
dihydrate was used as the anode catalyst instead of platinum black, the energy efficiency increased by 40% and the current density showed a 2-fold improvement.
Chapters 4, 5, and 6 focus on developing active Cu-based cathode catalysts for the
electroreduction of CO2 to C2 chemicals. Chapter 4 reports the synthesis and application of active
Cu nanoparticles with different morphology and composition (amount of surface oxide) for CO2
reduction in an alkaline electrolyzer. The use of catalysts with large surface roughness results in a high Faradaic efficiency of 46% (only ~30% in most prior work) for the conversion of CO2 to
C2 chemicals with a total current density of ~200 mA cm-2 for these C2 products, which, compared to prior work, represents a 10-fold increase in conversion rate at much lower overpotential (only < 0.7 V). The effect of N-containing compounds on the products distribution for the electroreduction of CO2 on Cu catalysts is discussed in Chapter 5. Specifically,
3,5-diamino-1,2,4-triazole (DAT) improves the Faradaic efficiency of C2H4 by more than 1.5 fold when used
Spectroscopy (SERS) was applied to elucidate the possible reasons for this improvement.
Chapter 6 describes the design, synthesis and application of CuPd nanoalloys with tunable atomic
arrangements (atomically ordered, disordered and phase-separated structures) for the electroreduction of CO2 to C2 chemicals. The results of electrochemical measurement as well as
structural and compositional characterization indicate that the observed differences in selectivities for different products can be attributed predominantly to structural differences in the different catalysts. Also, this work for the first time shows that active sites with neighboring Cu atoms are required for the efficient conversion of CO2 to C2 chemicals.
Finally, Chapter 7 describes the improvement in throughput levels for the electroreduction of CO2 to CO through the optimization of electrode structure and composition. The electrode that
incorporates multi-walled carbon nanotubes (MWCNTs) in the catalyst layer achieves high levels of CO production of up to 350 mA cm-2 at a high Faradaic efficiency (>95% selective for CO) and
an energy efficiency of 45%. This level of performance represents a twofold improvement over the performance achieved with electrodes that lack MWCNTs.
In summary the studies reported in this dissertation provide insight regarding the design and synthesis of active catalysts and electrodes that improve current density (conversion), selectivity and energy efficiency for the electroreduction of CO2 to different chemical
With outstanding professors, staff and experts, the Illini community has been an inspiring place to pursue research. I would like to express my gratitude to the many people who have helped to make this dissertation possible. First and foremost, I would like to thank my advisor, Professor Paul J.A. Kenis for providing insightful feedback and guidance for my research, and being extremely supportive of the research that I am interested in and would like to pursue. I also would like to thank my committee, Professors Andrew Gewirth, Catherine Murphy, Joaquín Rodrí guez-López for the advice and insight they provided.
I would like to thank all Kenis group members for being such great people to work with. First, I would like to thank Dr. Michael Thorson and Dr. Huei-Ru “Molly” Jhong, who demonstrated great patience when providing mentorship. I also would like to thank Byoungsu Kim, Sumit Verma, who I worked most closely with and helped to assume responsibilities for CO2
subgroup-related affairs. Joseph Whittenberg, Vivek Kumar, and Jeremy Schieferstein joined the same year as I did and I appreciated their comradery in lab and having me involved in ChBE activities. I am also grateful for the other members of the Kenis group for their scientific insight and comradery, particularly, Elizabeth Horstman, Dr. Amit Desai, Dr. Ashtamurthy Pawate, Dr. Matthew Byrne, Dr. Ritika Mohan, Dr. Sachit Goyal, Dr. Sudipto Guha, Dr. Matthew Naughton, Dr. Daria Khvostichenko, Dr. Joshua Tice, Dr. Adam Hollinger, and Dr. Jieqian Zhang. I also would like to thank exchange students that worked with me when they visited UIUC: Gaby Perez, Dr. Yangchun Lan, Dr. Sho Kitano and Lin Liu. Finally, I would like to thank hard working undergraduate researchers, Saman Moniri, Raymond Luo, Jake Gold and Aaron Yu, for their efforts in collecting data.
I have also been fortunate to interact with some wonderful faculty, students, and staff as collaborators both here and at Kyushu University. Without them, much of this work would not have been possible. Professor Andrew Gewirth has been a great mentor during these years and I am grateful for his guidance. His students, Dr. Claire Tornow, Kevin Schmitt and Thao Hoang worked very closely with me and offered a lot of help. I also would like to thank several great scientists and collaborators in Japan: Professors Miho Yamauchi, Masaaki Sadakiyo, Stephen Lyth, Naotoshi Nakashima, and Tsuyohiko Fujigaya at Kyushu University and Professor Teruhisa Ohno at Kyushu Institute of Technology.
I appreciate the generous funding for this work by DOE, Dioxide Materials, the U.S. Air Force, the International Institute for Carbon Neutral Energy Research (WPI-I2CNER, sponsored by the Japanese Ministry of Education, Culture, Sports, Science and Technology), as well as a Fellowship from FMC.
I appreciate my parents for mental support while I am away from home. I especially thank my friends here for making me feel like home.
Table of Contents
Chapter 1 Introduction... 1
1.1 Global Warming and the Need to Decrease Carbon Dioxide Emission ...1
1.2 Challenges in Energy ...3
1.3 Electroreduction of CO2 ...8
1.4 Current Status, Challenges and Future Opportunities of CO2 Reduction ...11
1.5 Summary and Thesis Outline ...16
1.6 References ...17
Chapter 2 Titania Supported Silver Catalyst for the Electroreduction of CO2 ... 22
2.1 Chapter Overview ...22
2.2 Introduction ...22
2.3 Experimental ...27
2.4 Results and Discussion ...30
2.5 Conclusions ...43
2.6 Supporting Information ...44
2.7 References ...50
Chapter 3 Effect of Anode Catalyst on the Electroreduction of CO2 ... 54
3.1 Chapter Overview ...54
3.2 Introduction ...54
3.3 Experimental ...57
3.5 Conclusions ...74
3.6 Supporting Information ...76
3.7 References ...79
Chapter 4 Cu Nanoparticles as Catalyst for Conversion of CO2 to C2 Products ... 83
4.1 Chapter Overview ...83
4.2 Introduction ...84
4.3 Experimental ...86
4.4 Results and Discussion ...91
4.5 Conclusions ...101
4.6 Supporting Information ...103
4.7 References ...105
Chapter 5 N-containing Compound for Efficient Reduction of CO2 to Ethylene... 109
5.1 Chapter Overview ...109
5.2 Introduction ...110
5.3 Experimental ...111
5.4 Results and Discussion ...115
5.5 Conclusions ...133
5.6 Supporting Information ...134
5.7 References ...137
Chapter 6 Bimetallic CuPd Catalysts for the Electroreduction of CO2 ... 140
6.1 Chapter Overview ...140
6.2 Introduction ...141
6.4 Results and Discussion ...147
6.5 Conclusions ...154
6.6 Supporting Information ...155
6.7 References ...158
Chapter 7 The Effect of Catalyst Layer Structure on CO2 Reduction ... 160
7.1 Chapter Overview ...160
7.2 Introduction ...161
7.3 Experimental ...163
7.4 Results and Discussion ...166
7.5 Conclusions ...176
7.6 References ...176
1.1 Global Warming and the Need to Decrease Carbon Dioxide Emission
In the past few decades, the atmospheric carbon dioxide (CO2) levels have increased
drastically (Figure 1.1) and are expected to continue to rise. In December 2015, the globally average mole fractions of CO2 reached 401.85 ppm,1 which is an increase of 44% compared to
pre-industrial levels (pre 1750).2 These high atmospheric CO2 levels are mainly attributed to
increased human activities such as fossil fuel combustion, cement production and flaring.3
Figure 1.1 Atmospheric CO2 concentrations from 1960 to present. The red curve represents
monthly mean data, while the black curve represents the seasonally corrected data. All the data was measured at Mauna Loa Observatory, Hawaii. Source: National Oceanic & Atmospheric Administration (NOAA), http://www.esrl.noaa.gov/gmd/ccgg/trends/full.html.
* Part of this work has been published: Jhong, H.-R. M., Ma, S. & Kenis, P. J. A. Electrochemical conversion of
CO2 to useful chemicals: current status, remaining challenges, and future opportunities. Curr. Opin. Chem. Eng. 2, 191-199, (2013). Copyright 2013. Reproduced with permission from Elsevier.
Carbon dioxide is the most important atmospheric greenhouse gas, which contributes ~65% of radiative forcing among all long-lived greenhouse gases. CO2 is responsible for ~84%
of the increase in radiative forcing from year 2004 to year 2013. Measurement of global surface temperatures over the past hundred years (Figure 1.2) indicates that the global climate is warming.4 As the Intergovernmental Panel on Climate Change (IPCC) states in their 2014 Synthesis Report,3 the increasing atmospheric concentrations of greenhouse gases are “extremely likely” to have been the dominant cause of the observed warming since the mid-20th century.
Figure 1.2 Global surface temperatures relative to 1880–1920 mean. Reprinted with permission
from ref 4. Copyright 2013 PLOS.
Already this high level of CO2 impacts the climate and global ecosystems in undesirable
ways as is evident from increasing sea levels, shifting climate zones, acidifying oceans, changing wildlife populations, and erratic weather patterns. These facts have caused increased pressure to rapidly decrease carbon emissions to restore Earth’s energy and carbon balance.4 The European Union and IPCC proposed to limit global warming to 2 °C relative to pre-industrial times to minimize deleterious consequences.5 To curb the rise, and eventually to lower the atmospheric CO2 levels, multiple approaches are proposed to be applied to reduce CO2 emissions include
and sequestration from point sources such as power plants, enhancing the energy efficiency of buildings and cars, and the utilization of renewable sources such as solar and wind.6 Increasing
the utilization of CO2, through both reductive and non-reductive pathways, is also proposed as it
can create economic value while helping to decrease atmospheric CO2 levels.7 Possible ways to
utilize CO2 as a feedstock for chemical production are shown in Figure 1.3. The first group of
methods forms products in which carbon keeps its +4 oxidation state: urea, polymeric materials, and inorganic carbonates. The second group aims to form products in which the oxidation state of carbon is reduced to +2 or lower: HCOOH, CO, C2H4, CH3OH, or CH3CH2OH. Compared to the
first group, formation of products within the second group requires higher energy exchange, which can be provided by strong reducing reagents, electricity, heat and/or radiation.7
Figure 1.3 Possible ways to utilize CO2 as a feedstock for chemical production.7 Redrawn with
permission from ref 7. Copyright 2015 RSC.
1.2 Challenges in Energy
Access to reliable and affordable energy has helped push the world towards more economic prosperity and has made human life better. However, as mentioned above, higher levels of prosperity have brought the problem of rising levels of greenhouse gasses to the atmosphere. Economic growth and energy-related emissions are coupled and move in the same direction
(Figure 1.4),8 as more than 80% of the energy we use today are from fossil fuels that emit greenhouse gases (mainly CO2).
Figure 1.4 (a) Evolution of primary energy shown as absolute contributions by different energy
sources (EJ); Reprinted with permission from ref 9. Copyright 2012 International Institute for Applied Systems Analysis. (b) World average GDP per capita 1500 to 2003. Source: https://commons.wikimedia.org/wiki/File:World_GDP_per_capita_1500_to_2003.png. data extracted from Angus Maddison's "World Population, GDP and Per Capita GDP, 1-2003 AD".
With the population continuing to increase, the world will consume much more energy than it does today in the next 20-30 years.10 The projected world energy consumption in 2040 will be about 40% more than today’s level (Figure 1.5),11 with most of the increase from
non-Organisation for Economic Co-operation and Development (non-OECD) countries. Therefore, finding ways to supply the rapidly increasing demand for energy while also limiting and/or decreasing carbon emissions is a major global challenge.
Figure 1.5 World energy consumption (in quadrillion Btu), 1990-2040. Reprinted with permission
In response to the need to meet the increasing energy demand while limiting greenhouse gas emissions, the International Energy Agency (IEA) proposed five energy sector measures: (1) increasing energy efficiency in the industry, building, and transport sectors; (2) progressively reducing the use of the least-efficient coal-fired power plants and banning their construction; (3) increasing investment in renewable energy to $400 billion in 2030; (4) gradually phasing out subsidies to fossil-fuel consumption; and (5) reducing methane emissions from oil and gas production.8 Many governments have already taken measures to promote these approaches. For
example, the United States, the European Union, China and Southeast Asia countries have set new energy performance standards for residential appliances such as refrigerators and air-conditioners to improve energy efficiency; China established a target of phasing out 10 gigawatts (GW) of small thermal power plants by 2020; Several countries have already announced reforms to fossil-fuel consumption subsidies; The United States has set a target to cut methane emissions from the oil and gas sector by 40% to 45% in 2025 relative to the levels of 2012; About $270 billion was invested in renewable energy development in the power sector in 2014 around the world.8 The global energy-related greenhouse gas emissions reduction achieved by these five policy measures in the Bridge Scenario (The Bridge Scenario depends upon the five proposed measures) relative to the INDC Scenario (Intended Nationally Determined Contributions Scenario: a first assessment of the impact of INDCs national pledges on the energy sector) is shown in Figure 1.6. In the INDC Scenario, national pledges have a positive impact in slowing the growth in global energy-related emissions, but emissions will still continue to rise. Effective implementation of the proposed measures in the Bridge Scenario will have a more profound effect on the global greenhouse gas emissions: Global emissions will be 4.8 Gt (or 13%) lower than in the INDC
Scenario by 2030. In the Bridge Scenario, energy related greenhouse gas emissions will peak and then begin to decline by around 2020.8
Figure 1.6 Global energy-related greenhouse gas emissions reduction by policy measure in the
Bridge Scenario relative to the INDC Scenario. Reprinted with permission from ref 8. Copyright 2015 International Energy Agency.
Among the five measures in the Bridge Scenario, contributions from investment in renewables for reduction of energy-related greenhouse gas emissions will be the second largest. The renewables, especially wind and solar, are becoming increasingly competitive in the market due to cost reduction. The average investment costs for solar panels, has fallen by a factor of more than four over the past few years in China and by a factor of two in the OECD;8 Wind turbine prices remained well below levels seen several years ago, while the turbine technology have improved significantly.12 Wind and solar energy production have accounted for more than 60% of the total global renewables-based power capacity additions in 2014.8 In the US, because federal
tax incentives are available for projects that initiated construction by the end of 2014, a further resurgence in new builds of wind turbines is anticipated in both 2015 and 2016.8 Therefore, further increasing contributions to power capacity from renewable sources such as wind and solar will continue.
However, wind and solar are intermittent sources, and often unpredictable. The electrical grid, by far the largest market for wind and solar energy, is not able to handle the intermittent nature of the rate by which they are produced. Customers still need electricity when the sun is not shining and the wind is not blowing. At times the electricity from wind and solar exceeds actual demand, and in the absence of large scale storage capacity is being wasted. The intermittency of wind and solar energy, therefore, hinders the economic competitiveness of those resources, as they are not necessarily available when they would be of greatest value to the system. As a result, methods for large-scale storage or on-demand utilization of intermittent electricity need to be developed so that lots of solar or wind energy can be stored and/or utilized when the supply is high.
Several approaches such as battery, pumped hydroelectric storage, electrolysis have been proposed to store excess intermittent renewable energy. In these approaches, electricity is converted to some other form of energy such as chemical energy or potential energy. Based on the type of battery used, it costs between 30 – 80 cents to store a kilowatt-hour of electricity.10 This cost is at least triple the price of electricity, which costs only 10 cents per kilowatt-hour on average in the US. Also, today’s batteries have much lower energy density than fossil fuels (about 30-70 times lower). Hydroelectric energy is currently widely used to store excess electricity in mountainous areas, while it cannot be used in flat areas such as the Midwest in the US. Storing electricity in a chemical form through electrolysis adds flexibility as electrolysis can be conducted where excess renewable energy is available, and the products such as hydrogen or liquid fuels can be used as sources for electricity and transportation fuels, or as a feedstock for chemical production.
1.3 Electroreduction of CO2
Among various electrolysis approaches, the electroreduction of CO2 into value-added
products such as formic acid, CO, hydrocarbons, or alcohols can store on demand excess renewable electricity in a chemical form, and thus at the same time it can help to reduce atmospheric CO2 levels. Figure 1.7 summarizes the main concept for the electroreduction of CO2.
If the chemical industry were CO2-based, the amount of CO2 that would be consumed yearly is
300 million metric tons.13 Also, compared to the traditional way of deriving chemicals from fossil
fuels, the electroreduction of CO2 does not rely on fossil fuels and is thus a more sustainable
approach as long as it uses electricity from renewable sources or at least from a carbon-neutral source.
Figure 1.7 Schematic overview of the electroreduction of CO2. Redraw with permission from ref
14. Copyright 2013 Elsevier.
The electrochemical conversion of CO2 to other compounds is realized by reducing CO2
using electrons in the electrical circuit as the driving force for the necessary uphill reactions. In an electrolyzer, CO2 is reduced on the cathode while a compensating reaction such as the oxygen
of the cathode for the electroreduction of CO2 into major products such as CO, formic acid,
methane, ethylene, and ethanol are listed in Table 1.1. Another important reaction that happens during the CO2 reduction process is the hydrogen evolution reaction (HER) when an aqueous
solution is used as the electrolyte. The standard electrode potential of hydrogen evolution reaction (HER) is 0 V vs. RHE, which is in the similar standard potential ranges for the CO2 reduction
reaction. Therefore, H2 is often a major byproduct during CO2 reduction.16
Table 1.1 Major half-cell reactions for the electroreduction of CO2.
Reaction E˚ (V) (vs. RHE)
CO2 + H2O + 2e- CO + 2OH- -0.10
CO2 + H2O + 2e- HCOO- + OH- -0.02
CO2 + 6H2O + 8e- CH4 + 8OH- +0.17
2CO2 + 8H2O + 12e- C2H4 + 12OH- +0.08
2CO2 + 9H+ + 12e- C2H5OH + 3OH- +0.09
The process of CO2 electrolysis is basically running a fuel cell in reverse; so indeed, many
lessons learned over the last five or so decades in the development of catalysts, electrodes and cell configurations for fuel cells do apply also to the development of efficient CO2 processes, but
certain aspects will be very different and will require different optimization strategies. For example, both low-temperature fuel cells and CO2 electrolysis cells are often limited by cathode
performance, so both seek to improve slow cathode kinetics by developing more active catalysts. However, in addition to activity, catalysts for CO2 reduction need to exhibit high product
selectivity so the formation of desired products is heavily favored over unwanted reactions. Moreover, effective removal of products from the catalyst layer to avoid blocking active sites is important in both fuel cells and CO2 electrolysis cells, but the technical strategies to do so can be
in acidic fuel cells generates water which often leads to water management issues, whereas the CO2 reduction reaction in CO2 electrolysis cells often leads to the formation of both gaseous (e.g.,
CO, H2) and liquid products and thus effective gas / liquid phase separation is vital.
For electroreduction of CO2 to be performed in an efficient manner, highly active and
durable electrocatalysts for both the cathode (CO2 reduction reaction) and the anode (O2 evolution
reaction), as well as electrodes and electrolytes that have high conductivity and allow for sufficient mass transport of the reactants and products to/from the catalyst layers are required. Key figures of merit of the process that characterize its performance and thus assist in determining its economic feasibility are (i) the Energy Efficiency (EE) – a measure of the overall energy utilization towards the desired product; (ii) the Current Density (CD) – a measure of the rate of conversion; (iii) the Faradaic Efficiency (FE) – a measure of the selectivity of the process for a given product; (iv) the catalyst stability; and (v) process costs17 – including material consumption costs, capital cost and
electricity cost. This dissertation will focus on the first three figures of merit (EE, FE, and CD) because currently neither standard protocols for durability tests of catalysts nor cost models for major products exist for electrochemical CO2 conversion.
The energy efficiency can be calculated using equation 1:
k k Faradaic , k k energetic E E (1)
where Ek is the equilibrium cell potential for a certain product. For example, Eo = Eo
cathode - Eoanode
= -0.10 V - 1.23 V = -1.33 V for converting CO2 to CO and Eo = Eocathode - Eoanode = 0 V - 1.23 V
= -1.23 V for H2 evolution). k ,Faradaic is the Faradaic efficiency of product k and is the cell
overpotential (or the sum of overpotentials on the cathode and anode). From this equation it becomes clear that high energy efficiency is achieved through a combination of high Faradaic
efficiency for the desired product, and low overpotentials on the cathode and anode, because that will lead to a low cell potential. Note that at times researchers use a slightly different approach to determine the energy efficiency of their experimental setup.18
The Faradaic efficiency (sometimes also referred to as the current efficiency) for a given product is calculated using equation 2:
Q F n z Faradaic (2)
where z is the number of electrons exchanged (for example, n = 2 for reduction of CO2 to CO),
the number of moles for a given product, F Faraday‘s constant (F = 96485 C/mol), and Q the charge passed (C).15,18,19
The overall current density, defined as the current at a given cell potential divided by the active cathode electrode area (geometric surface area of the cathode), is a measure of the electrochemical reaction rate (conversion), so it helps determine the electrode area (and thus the electrolyzer size and capital investment) needed to meet the desired rate of producing the product. One can also calculate partial current densities for the individual products formed by multiplying overall current density by the corresponding FE.
1.4 Current Status, Challenges and Future Opportunities of CO2 Reduction
In addition to providing opportunities to curb atmospheric CO2 levels and store intermittent
renewable energy, the electroreduction of CO2 also has the potential for economic gains as it
produces valuable chemicals or fuels. However, to make this process viable for commercialization, significant improvements in energy efficiency, current density and product selectivity are needed. In this whole process, catalysts, electrodes, electrolytes, as well as reactors (electrolyzers) play important roles in determining the energy efficiency, current density and
product selectivity. (1) Electrocatalysts and (2) electrolytes largely determine kinetics, thereby affecting all the figures of merit; (3) Reactors influence the mass transportation of reactants and products, thereby affecting the current density mostly; (4) Electrodes determine the electron conductivity and mass transportation to/from catalysts, thereby majorly affecting energy efficiency and current density. Current combinations of catalysts, electrodes, electrolytes and reactors have not rendered the electroreduction of CO2 with similar performance as already commercialized
electrolysis technology, e.g., water electrolysis and chlor-alkali process. Therefore, both challenges and opportunities exist within these four areas of research to further improve the viability of CO2 reduction for being practically applied.
Electrocatalysts are needed to bind and activate CO2 in order to reduce the high
overpotentials typically encountered. Also, catalysts can drive selective formation of desired products. During the past few decades efforts have mostly focused on different metal catalysts and the various products that can be formed using those metals.20-23 Four distinct classes of metal catalysts have been identified for CO2 reduction: (1) metals that mainly form formic acid, HCOOH
(Pb, Hg, In, Sn, Cd, Tl); (2) metals that mainly form carbon monoxide, CO (Au, Ag, Zn, Pd, Ga); (3) metals that form significant amounts of hydrocarbons such as methane and ethylene (Cu); and (4) metals that mainly form H2 (Pt, Ni, Fe, Ti).20 Other potential products formed using metal
catalysts include alcohols24 and oxalic acid25. Over the last few years, researchers have also started to study other materials, including metal oxides26-29, roughened or nanostructured metal
catalysts,30-33 metal organic frameworks (MOF),34 covalent organic frameworks,35 pyridine related organic compounds36,37 as well as organometallic catalysts.38 The chemistries between the catalyst
and the reactant/intermediates were investigated using either spectroscopic techniques39,40 or computational approaches such as DFT41-43 to reveal structure-activity relationships.
Catalysts that simultaneously exhibit low overpotentials (e.g., < -0.2 V) and high current densities (e.g., >100 mA/cm2) needed for commercial applications are still lacking. The quest for such catalysts could be aided by (i) more fundamental studies focusing on elucidation of reaction mechanisms for distinct catalysts, an area in which reports are few42,44,45, and (ii) more in-depth modeling efforts, ideally linked directly with experimental work, so pathways for CO2 reduction
on different catalysts can be better understood, which in turn will assist the design and synthesis of novel catalysts that have both low overpotential and high activity for CO2 reduction reactions.
The above-mentioned recent reports in this section on a variety of promising catalysts for CO2
reduction (MOFs, organometallics, etc.) suggest that significant strides will be made to enhance catalyst activity while reducing overpotential. Such efforts will greatly benefit from fundamental mechanistic studies, as well as modeling of new classes of catalytic materials.
Electrodes play a vital role in all devices based on heterogeneous electrochemical reactions, including those for CO2 conversion. The performance and durability of the reactor is largely
determined by the processes occurring at the electrode-electrolyte interface and within the electrode. Maximizing electrode performance, and consequently reactor performance, requires optimizing all of these transport processes that strongly depend on the complex structure of the electrode. Despite their importance, to date only a few efforts have studied the interplay between electrode structure and performance.18,20,46-48 In early work, Hori et al. extensively studied the CO2 reduction reaction on planar metal electrodes (Cu, Au, Ag, Zn, Pd, Ga, Pb, Hg, In, Sn, Cd,
concentrations at the electrode surface due to the limited CO2 solubility in the aqueous electrolytes
used limits the performance of such planar electrodes. Recently, Delacourt et al. hand- or spray-painted Ag catalyst inks on gas diffusion layers (GDLs) to generate cathodes with a Ag (particle size of 1 µm) loading of 8-10 mg/cm2.18 This Ag nanoparticle-covered GDE (cathode) achieved current densities as high as 20 mA/cm2, in combination with product selectivities for CO and H2
that are comparable to the findings by Hori et al.20 and Yano et al.46 using similar catalysts (Ag) and electrolytes (0.5 M KHCO3). Our lab recently developed a fully-automated airbrushing
method to deposit a very thin, crack free layer with a Ag loading of only 0.75 mg/cm2.48 The electrolyzer equipped with this kind of electrode achieved a current density as high as 91 mA/cm2 in combination with 94% Faradaic efficiency for CO, and 46% energy efficiency. Use of a GDE in combination with optimized catalyst layer deposition methods has led to significant improvement in electrode performance for CO2 reduction. Further efforts should probably focus
on assessing, via experiment and modeling, to what extent the structure and chemical composition of the catalyst layer (e.g., pore size and distribution, the choice of binder materials such as Nafion) and the porous backing layer (e.g., porosity, hydrophobicity, layer thickness) impact the transport of reactants (sufficient supply of CO2?) and products (active sites blocked?).
Electrolytes have been known to affect almost every electrochemical process dating back to the days of Frumkin.49 The heterogeneous electrochemical reduction of CO2 employs aqueous
electrolytes commonly comprised of alkali cations (e.g., Na+, K+), various anions such as halide anions (e.g., Cl-), bicarbonate (HCO3-), or hydroxide (OH-), and water.20,50-52 These inorganic salts
are often used due to their high conductivities in water. Additionally, the water in aqueous electrolytes provides protons for the necessary electrochemical proton transfer steps involved in
the reaction pathway.20,42 A number of prior reports have shown that electrolyte choice has profound effects on current density, product selectivity, and energy efficiency in CO2 reduction.50
For example, Hori et al. reported that cation choice (i.e., Li+, Na+, K+, and Cs+) for bicarbonate (HCO3-) electrolytes significantly impacts the distribution of product formed on copper (Cu)
electrodes.50-52 Hori et al. also reported that anion choice (i.e., Cl-, ClO4-, SO4-, HCO3-, H2PO4-),
each with different buffer capacities, influences the local pH at the Cu electrode and thus the nature and the amount of products formed.51 Similar to these findings by Hori et al., Wu et al. observed
significant differences in activity and selectivity of tin (Sn) electrodes when different electrolytes (KHCO3, K2SO4, KCl, Na2SO4, Cs2SO4, NaHCO3, and CsHCO3) are used.52 Previously, we
reported that the size of the cation (Na+ < K+ < Rb+ < Cs+) of the salt used in the electrolyte plays a significant role in CO2 reduction on silver (Ag) electrodes. Specifically, larger cations favor CO
production and suppress H2 evolution.53 In summary, these studies show that (i) cation size
impacts the propensity for cation adsorption on the electrode surface, which affects the potential of the outer Helmholtz plane (OHP) in the electrical double layer (EDL), and in turn impacts reaction energetics and kinetics; and (ii) the buffer capacity of anions impacts the local pH at the electrode and thus the availability of protons, which in turn affects reaction kinetics. Furthermore, depending on reactor configuration, electrolyte composition may enhance performance by improving the solubility of CO2, for instance by using ionic liquids54 instead of aqueous solution,
thereby reducing mass transport limitations.
No standard experimental setup or methodology for studying electrochemical CO2
reduction currently exists. Different labs have used a variety of flow cells or electrolyzers for the various studies reported here. Jaramillo and coworkers,15 as well as our lab,38,48,53,55 use a
microfluidic flow cell in which the electrodes are separated by a flowing liquid electrolyte, which enables analysis of individual electrode performance by using an external reference electrode. Delacourt et al. based their design on an alkaline fuel cell,18 while Dufek et al. used a more traditional electrolyzer design.56-59 Interestingly, three of these systems exhibit similar behavior when comparing their performance for CO production. Indeed, Dufek et al.56,59 have reported improved reactor performance at elevated temperature and/or pressure. Further optimization of operating conditions (e.g., electrolyzers operated at elevated pressure and temperature) will continue to improve reactor performance in CO2 reduction. Specifically, multiple labs have
reported enhanced current densities in pressurized electrolyzers (e.g., 20 atm).60,61 For example, Furuya et al. reported that a total current density as high as 300-900 mA/cm2 can be achieved under 20 atm using a pressurized electrolyzer operated with GDEs coated with different metals (Pt, Ag, Cu, Ni, Co, Pd).60
1.5 Summary and Thesis Outline
In summary, the electroreduction of CO2 shows promise to store intermittent renewable
energy in the form of chemical bonds and reduce carbon emissions. However, to be used commercially, improvements are needed regarding the present low energy efficiency and current density of the reaction. The purpose of this dissertation is to develop active catalysts and proper electrode structures to improve the current density and selectivity to certain products, thereby improving the energy efficiency for the electroreduction of CO2. This dissertation will also discuss
insights into CO2 reduction reaction gained through studying the activity of various catalysts with
different structures or properties. Hopefully the insight gained will help guide the design of better catalysts and electrodes for this process.
Specifically, Chapters 2, 3 and 7 focus on improving the current density and the energy efficiency for the electroreduction of CO2 to CO. Chapter 2 presents the use of a support material
to lower the Ag-based cathode catalyst loading without sacrificing performance. Chapter 3 discusses how improvements to the anode can drastically improve the prospects of the electrochemical reduction of CO2. Chapter 7 details the design and application of Ag cathodes
with the incorporation of multi-walled carbon nanotubes to improve the current density and energy efficiency. Chapters 4, 5 and 6 mainly focus on developing Cu-related catalysts to improve the production of C2 chemicals (ethylene and ethanol) from CO2. Chapter 4 explores the application
of Cu nanoparticles with different morphologies for the efficient conversion of CO2 to C2 products.
Chapter 5 demonstrates the use of N-containing ligand to improve the selectivity to C2 chemicals on Cu-based catalysts. Chapter 6 discusses the effect of bimetallic alloy structures on the production of C2 chemicals.
1 Tans, P. & Keeling, R. Recent Monthly Average Mauna Loa CO2. (ESRL Global
Monitoring Division Global Greenhouse Gas Reference Network. URLL: http://www.esrl.noaa.gov/gmd/ccgg/trends/, 2015).
2 Astor, Y., Bates, N., Church, M., Coppola, L., Currie, K., González-Dávila, M., Miller, L., Nakano, T. & Wakita, M. WMO Greenhouse Gas Bulletin. 8 (World Meteorological Organization, 2014).
3 Pachauri, R. K. & Meyer, L. Climate Change 2014: Synthesis Report. 151 (IPCC, Geneva, Switzerland, 2014).
4 Hansen, J., Kharecha, P., Sato, M., Masson-Delmotte, V., Ackerman, F., Beerling, D. J., Hearty, P. J., Hoegh-Guldberg, O., Hsu, S.-L., Parmesan, C., Rockstrom, J., Rohling, E. J., Sachs, J., Smith, P., Steffen, K., Van Susteren, L., von Schuckmann, K. & Zachos, J. C. Assessing “Dangerous Climate Change”: Required Reduction of Carbon Emissions to Protect Young People, Future Generations and Nature. PLoS One 8, e81648, (2013). 5 Randalls, S. History of the 2°C climate target. Wiley Interdisciplinary Reviews: Climate
Change 1, 598-605, (2010).
6 Pacala, S. & Socolow, R. Stabilization Wedges: Solving the Climate Problem for the Next 50 Years with Current Technologies. Science 305, 968-972, (2004).
7 Martin, A. J., Larrazabal, G. O. & Perez-Ramirez, J. Towards sustainable fuels and chemicals through the electrochemical reduction of CO2: lessons from water electrolysis. Green Chem. 17, 5114-5130, (2015).
8 Wanner, B., Kęsicki, F., Hood, C., Baroni, M., Bennett, S., Besson, C., Bouckaert, S., Bromhead, A., Durand-Lasserve, O., El-Laboudy, T., Gould, T., Hashimoto, M., Klingbeil, M., Kurozumi, A., Levina, E., Liu, J., McCoy, S., Olejarnik, P., Selmet, N., Sinopoli, D., Suehiro, S., Trüby, J., Vailles, C., Wilkinson, D., Zazias, G. & Zhang, S. Energy and Climate Change - World Energy Outlook Special Report 2015. 200 (International Energy Agency, Paris, France, 2015).
9 Banerjee, R., Benson, S. M., Bouille, D. H., Brew-Hammond, A., Cherp, A., Coelho, S. T., Emberson, L., Figueroa, M. J. n., Grubler, A., Jaccard, M., Ribeiro, S. K., Karekezi, S., He, K., Larson, E. D., Li, Z., McDade, S., Mytelka, L. K., Pachauri, S., Patwardhan, A., Riahi, K., m, J. R. ö., Rogner, H.-H., Roy, J., Schock, R. N., Sims, R., Smith, K. R., Turkenburg, W. C., rge-Vorsatz, D. Ü., Hippel, F. v. & Yeager, K. Global Energy Assessment - Toward a Sustainable Future. (2012).
10 Gates, B. Energy Innovation - Why We Need It and How to Get It. (2015).
11 Conti, J., Holtberg, P., Beamon, J. A., Napolitano, S., Schaal, A. M., Turnure, J. T., Westfall, L., Geagla, A., Grissom, S., Maples, J., Teller, K., Smith, K. A., Staub, J., Ayoub, J., Cheung, C., Eshbaugh, M., Griffin, K., Lou, J., Smith, P., Smith, C. L., Federhen, C. & Wells, P. International Energy Outlook 2013. 312 (U.S. Energy Information Administration, Washington DC, USA, 2013).
12 Wiser, R. & Bolinger, M. 2014 Wind Technologies Market Report. 93 (U.S. Department of Energy, 2015).
13 Scott, A. in Chem. Eng. News Vol. 93 7 (American Chemical Society, 2015).
14 Jhong, H.-R. M., Ma, S. & Kenis, P. J. A. Electrochemical conversion of CO2 to useful
chemicals: current status, remaining challenges, and future opportunities. Curr. Opin. Chem. Eng. 2, 191-199, (2013).
15 Kuhl, K. P., Cave, E. R., Abram, D. N. & Jaramillo, T. F. New insights into the electrochemical reduction of carbon dioxide on metallic copper surfaces. Energy Environ. Sci. 5, 7050-7059, (2012).
16 Hori, Y. in Modern Aspects of Electrochemistry Vol. 42 Modern Aspects of Electrochemistry (eds ConstantinosG Vayenas, RalphE White, & MariaE Gamboa-Aldeco) Ch. 3, 89-189 (Springer New York, 2008).
17 Oloman, C. & Li, H. Electrochemical Processing of Carbon Dioxide. ChemSusChem 1, 385-391, (2008).
18 Delacourt, C., Ridgway, P. L., Kerr, J. B. & Newman, J. Design of an Electrochemical Cell Making Syngas ( CO + H2 ) from CO2 and H2O Reduction at Room Temperature. J.
Electrochem. Soc. 155, B42-B49, (2008).
19 Wu, J., Risalvato, F. & Zhou, X.-D. Effects of the Electrolyte on Electrochemical Reduction of CO2 on Sn Electrode. ECS Trans. 41, 49-60, (2012).
20 Hori, Y., Wakebe, H., Tsukamoto, T. & Koga, O. Electrocatalytic Process of CO Selectivity in Electrochemical Reduction of CO2 at Metal-Electrodes in Aqueous-Media.
Electrochim. Acta 39, 1833-1839, (1994).
21 Azuma, M., Hashimoto, K., Hiramoto, M., Watanabe, M. & Sakata, T. Electrochemical Reduction of Carbon-Dioxide on Various Metal-Electrodes in Low-Temperature Aqueous KHCO3 Media. J. Electrochem. Soc. 137, 1772-1778, (1990).
22 Hori, Y., Kikuchi, K. & Suzuki, S. Production of CO and CH4 in Electrochemical
Reduction of CO2 at Metal-Electrodes in Aqueous Hydrogencarbonate Solution. Chem.
Lett., 1695-1698, (1985).
23 Ikeda, S., Takagi, T. & Ito, K. Selective Formation of Formic-Acid, Oxalic-Acid and Carbon-Monoxide by Electrochemical Reduction of Carbon-Dioxide. Bull. Chem. Soc. Jpn. 60, 2517-2522, (1987).
24 Hori, Y. in Handbook of Fuel Cells Vol. 2 Ch. 48, 720-733 (John Wiley & Sons, Ltd, 2010).
25 Tomita, Y., Teruya, S., Koga, O. & Hori, Y. Electrochemical reduction of carbon dioxide at a platinum electrode in acetonitrile-water mixtures. J. Electrochem. Soc. 147, 4164-4167, (2000).
26 Chen, Y., Li, C. W. & Kanan, M. W. Aqueous CO2 Reduction at Very Low Overpotential
on Oxide-Derived Au Nanoparticles. J. Am. Chem. Soc. 134, 19969-19972, (2012). 27 Li, C. W. & Kanan, M. W. CO2 Reduction at Low Overpotential on Cu Electrodes
Resulting from the Reduction of Thick Cu2O Films. J. Am. Chem. Soc. 134, 7231-7234,
28 Chen, Y. H. & Kanan, M. W. Tin Oxide Dependence of the CO2 Reduction Efficiency on
Tin Electrodes and Enhanced Activity for Tin/Tin Oxide Thin-Film Catalysts. J. Am. Chem. Soc. 134, 1986-1989, (2012).
29 Ren, D., Deng, Y., Handoko, A. D., Chen, C. S., Malkhandi, S. & Yeo, B. S. Selective Electrochemical Reduction of Carbon Dioxide to Ethylene and Ethanol on Copper(I) Oxide Catalysts. ACS Catal. 5, 2814-2821, (2015).
30 Roberts, F. S., Kuhl, K. P. & Nilsson, A. High Selectivity for Ethylene from Carbon Dioxide Reduction over Copper Nanocube Electrocatalysts. Angew. Chem. 127, 5268-5271, (2015).
31 Tang, W., Peterson, A. A., Varela, A. S., Jovanov, Z. P., Bech, L., Durand, W. J., Dahl, S., Norskov, J. K. & Chorkendorff, I. The importance of surface morphology in controlling the selectivity of polycrystalline copper for CO2 electroreduction. Phys. Chem. Chem.
Phys. 14, 76-81, (2012).
32 Lu, Q., Rosen, J., Zhou, Y., Hutchings, G. S., Kimmel, Y. C., Chen, J. G. & Jiao, F. A selective and efficient electrocatalyst for carbon dioxide reduction. Nat. Commun. 5, (2014).
33 Ma, S., Sadakiyo, M., Luo, R., Heima, M., Yamauchi, M. & Kenis, P. J. A. One-step electrosynthesis of ethylene and ethanol from CO2 in an alkaline electrolyzer. J. Power
Sources 301, 219-228, (2016).
34 Hinogami, R., Yotsuhashi, S., Deguchi, M., Zenitani, Y., Hashiba, H. & Yamada, Y. Electrochemical Reduction of Carbon Dioxide Using a Copper Rubeanate Metal Organic Framework. ECS Electrochemistry Letters 1, H17-H19, (2012).
35 Lin, S., Diercks, C. S., Zhang, Y.-B., Kornienko, N., Nichols, E. M., Zhao, Y., Paris, A. R., Kim, D., Yang, P., Yaghi, O. M. & Chang, C. J. Covalent organic frameworks comprising cobalt porphyrins for catalytic CO2 reduction in water. Science 349,
36 Barton Cole, E., Lakkaraju, P. S., Rampulla, D. M., Morris, A. J., Abelev, E. & Bocarsly, A. B. Using a One-Electron Shuttle for the Multielectron Reduction of CO2 to Methanol:
37 Barton, E. E., Rampulla, D. M. & Bocarsly, A. B. Selective Solar-Driven Reduction of CO2 to Methanol Using a Catalyzed p-GaP Based Photoelectrochemical Cell. J. Am. Chem.
Soc. 130, 6342-6344, (2008).
38 Tornow, C. E., Thorson, M. R., Ma, S., Gewirth, A. A. & Kenis, P. J. A. Nitrogen-Based Catalysts for the Electrochemical Reduction of CO2 to CO. J. Am. Chem. Soc. 134,
39 García Rey, N. & Dlott, D. D. Structural Transition in an Ionic Liquid Controls CO2
Electrochemical Reduction. J. Phys. Chem. C 119, 20892-20899, (2015).
40 Schmitt, K. G. & Gewirth, A. A. In Situ Surface-Enhanced Raman Spectroscopy of the Electrochemical Reduction of Carbon Dioxide on Silver with 3,5-Diamino-1,2,4-Triazole. J. Phys. Chem. C 118, 17567-17576, (2014).
41 Montoya, J. H., Peterson, A. A. & Nørskov, J. K. Insights into C-C Coupling in CO2
Electroreduction on Copper Electrodes. ChemCatChem 5, 737-742, (2013).
42 Peterson, A. A., Abild-Pedersen, F., Studt, F., Rossmeisl, J. & Norskov, J. K. How copper catalyzes the electroreduction of carbon dioxide into hydrocarbon fuels. Energy Environ. Sci. 3, 1311-1315, (2010).
43 Peterson, A. A. & Nørskov, J. K. Activity Descriptors for CO2 Electroreduction to Methane
on Transition-Metal Catalysts. J. Phys. Chem. Lett. 3, 251-258, (2012).
44 Chandrasekaran, K. & Bockris, L. O. M. In-situ spectroscopic investigation of adsorbed intermediate radicals in electrochemical reactions: CO2− on platinum. Surf. Sci. 185,
45 Schouten, K. J. P., Qin, Z., Gallent, E. P. & Koper, M. T. M. Two Pathways for the Formation of Ethylene in CO Reduction on Single-Crystal Copper Electrodes. J. Am. Chem. Soc. 134, 9864-9867, (2012).
46 Yano, H., Shirai, F., Nakayama, M. & Ogura, K. Electrochemical reduction of CO2 at
three-phase (gas vertical bar liquid vertical bar solid) and two-phase (liquid vertical bar solid) interfaces on Ag electrodes. J. Electroanal. Chem. 533, 113-118, (2002).
47 Yano, H., Shirai, F., Nakayama, M. & Ogura, K. Efficient electrochemical conversion of CO2 to CO, C2H4 and CH4 at a three-phase interface on a Cu net electrode in acidic solution.
J. Electroanal. Chem. 519, 93-100, (2002).
48 Jhong, H.-R. M., Brushett, F. R. & Kenis, P. J. A. The Effects of Catalyst Layer Deposition Methodology on Electrode Performance. Adv. Energy Mater. 3, 589-599, (2013).
49 Frumkin, A. N. Influence of Cation Adsorption on the Kinetics of Electrode Processes. T Faraday Soc 55, 156-167, (1959).
50 Murata, A. & Hori, Y. Product Selectivity Affected by Cationic Species in Electrochemical Reduction of CO2 and CO at a Cu Electrode. Bull. Chem. Soc. Jpn. 64, 123-127, (1991).
51 Hori, Y., Murata, A. & Takahashi, R. Formation of hydrocarbons in the electrochemical reduction of carbon dioxide at a copper electrode in aqueous solution. J. Chem. Soc., Faraday Trans. 1 85, 2309-2326, (1989).
52 Wu, J., Risalvato, F. G., Ke, F.-S., Pellechia, P. J. & Zhou, X.-D. Electrochemical Reduction of Carbon Dioxide I. Effects of the Electrolyte on the Selectivity and Activity with Sn Electrode. J. Electrochem. Soc. 159, F353-F359, (2012).
53 Thorson, M. R., Siil, K. I. & Kenis, P. J. A. Effect of Cations on the Electrochemical Conversion of CO2 to CO. J. Electrochem. Soc. 160, F69-F74, (2013).
54 Rosen, B. A., Salehi-Khojin, A., Thorson, M. R., Zhu, W., Whipple, D. T., Kenis, P. J. A. & Masel, R. I. Ionic Liquid–Mediated Selective Conversion of CO2 to CO at Low
Overpotentials. Science 334, 643-644, (2011).
55 Whipple, D. T., Finke, E. C. & Kenis, P. J. A. Microfluidic Reactor for the Electrochemical Reduction of Carbon Dioxide: The Effect of pH. Electrochem. Solid-State Lett. 13, B109-B111, (2010).
56 Dufek, E. J., Lister, T. E., Stone, S. G. & McIlwain, M. E. Operation of a Pressurized System for Continuous Reduction of CO2. J. Electrochem. Soc. 159, F514-F517, (2012).
57 Dufek, E. J., Lister, T. E. & McIlwain, M. E. Influence of S Contamination on CO2
Reduction at Ag Electrodes. J. Electrochem. Soc. 158, B1384-B1390, (2011).
58 Dufek, E. J., Lister, T. E. & McIlwain, M. E. Influence of Electrolytes and Membranes on Cell Operation for Syn-Gas Production. Electrochem. Solid-State Lett. 15, B48-B50, (2012).
59 Dufek, E., Lister, T. & McIlwain, M. Bench-scale electrochemical system for generation of CO and syn-gas. J. Appl. Electrochem. 41, 623-631, (2011).
60 Furuya, N., Yamazaki, T. & Shibata, M. High performance Ru-Pd catalysts for CO2
reduction at gas-diffusion electrodes. J. Electroanal. Chem. 431, 39-41, (1997).
61 Sonoyama, N., Kirii, M. & Sakata, T. Electrochemical reduction of CO2 at metal-porphyrin
supported gas diffusion electrodes under high pressure CO2. Electrochem. Commun. 1,
Titania Supported Silver Catalyst for the Electroreduction of CO2
2.1 Chapter Overview
While significant research efforts have focused on the exploration of catalysts for electrochemical reduction of CO2, considerably fewer efforts have studied how support materials
for these catalysts affect their performance, including their ability to reduce the overpotential, and/or to increase the catalyst utilization and selectivity. Here Ag nanoparticles supported on carbon black (Ag/C) and on titanium dioxide (Ag/TiO2) were synthesized. In a flow reactor, 40
wt% Ag/TiO2 exhibited two-fold higher current density for CO production than 40 wt% Ag/C.
Faradaic efficiencies of the 40 wt% Ag/TiO2 catalyst exceeded 90% with a partial current density
for CO of 101 mA cm-2; similar to the performance of unsupported Ag nanoparticle catalysts (AgNP), but at a 2.5 times lower silver loading. A mass activity as high as 2700 mAmgAg-1cm-2
was achieved. In cyclic voltammetry (CV) in a three-electrode cell, Ag/TiO2 exhibited a lower
overpotential for CO2 reduction than AgNP, which, together with other data, suggests that TiO2
stabilizes the intermediate and serves as redox electron carrier to assist CO2 reduction while Ag
assists in formation of the final product CO.
The world’s increasing energy consumption due to increases in the world population and increased energy consumption in developing parts of the world, is accelerating the depletion of the
* Part of this work has been published: Ma , S., Lan , Y., Perez, G. M. J., Moniri, S. & Kenis , P. J. A. Silver Supported
on Titania as an Active Catalyst for Electrochemical Carbon Dioxide Reduction. ChemSusChem 7, 866-874, (2014). Copyright 2014. Reproduced with permission from Wiley.
world’s dwindling fossil fuel reserves.62,63 This increased energy consumption has led to a steady
increase in atmospheric CO2 levels over several decades, which in turn has been linked to
undesirable climate change effects. To curb the rise, and eventually to lower the atmospheric CO2
levels, multiple approaches need to be pursued, because no single approach has the capacity to address this issue by itself.6 Approaches to reduce CO2 emissions include switching to energy
sources that emit less CO2 (e.g., natural gas instead of coal), carbon capture and sequestration from
point sources such as power plants, enhancing the energy efficiency of buildings and cars, and the utilization of renewable sources such as solar and wind. Potential economic gains provide a natural incentive for the implementation of some of these approaches (e.g., enhancing energy efficiency of buildings and cars), whereas other approaches will require regulation as they can only be implemented at a substantial cost (e.g., carbon capture and underground sequestration). Many renewable power plants (wind, solar, tidal, etc.) have become operational around the world, but due to their intermittent nature these sources can only be used in combination with more conventional, fossil fuel based power plants. Furthermore, to avoid renewable power being wasted when the amount being produced is high, methods for large scale energy storage or on-demand utilization need to be developed.64,65
The catalytic conversion of CO2 into useful chemicals such as intermediates for the
synthesis of fuels and polymers using photochemical, electrochemical, thermochemical, or other methods is another promising approach to curb atmospheric CO2 levels, while at the same time
providing the potential for economic gains.17,24,66-71 More specifically, the electrochemical conversion of CO2 into value-added products, such as formic acid, carbon monoxide,
hydrocarbons, or alcohols can utilize on demand excess energy from renewable energy plants while simultaneously helping to reduce atmospheric CO2 levels.72 However, significant
improvements in the efficiency and at times the selectivity of the electrolysis of CO2 into any of
these products are needed for this process to become economically viable.16,72,73 Most
electrocatalysts reported to date exhibit a high overpotential for the desired reaction, which drastically reduces the energy efficiency. Also, conversion rate, as expressed by the observed current density, is still insufficient. Electrocatalysts need to be developed that simultaneously exhibit a low overpotential (thus high energy efficiency), high Faradaic efficiency (high selectivity), and high current density (thus high rate of conversion).14,72
Over the past decades multiple metal catalysts have been tested for the production of various products by electrochemical reduction of CO2.15,16,21-23,74 For example, Hori et al. found
that different metal catalysts exhibit selectivity for different products: i.e., metals such as Ag and Au lead to predominantly CO, metals such as Sn lead to formate while Cu leads to the formation of mixtures of hydrocarbons.20 Here, the conversion of CO
2 to CO is focused in this chapter since
the combination of CO and H2 (syngas) can be converted to liquid fuels through the
Fischer-Tropsch process. Although some catalysts are able to produce CO and H2 at the same time,
catalysts that predominantly produce CO are focused because H2 can be obtained more efficiently
(higher system efficiency and current density) from other sources, e.g. water electrolysis, than by co-generating H2 with CO. Overall, optimizing the electrolysis cell for CO production and
supplying H2 from water electrolysis will be energetically more efficient than co-generation in a
Some of the early work indicates that the large overpotential needed for CO2 reduction
mainly stems from the barrier of the initial electron transfer to form a CO2•- intermediate that is
poorly stabilized by most metal surfaces.24,44 Some approaches to stabilize this intermediate,
(1-Ethyl-3-methylimidazolium tetrafluoro-borate) as a co-catalyst in combination with unsupported Ag nanoparticle-based catalyst to lower the cell overpotential for the electroreduction of CO2 to CO on silver electrodes to ~0.2 V, although only at low current densities (<5 mA cm-2)
and high loading (6.67 mg of Ag per cm2).54 Chen et al. reduced the overpotential of CO2 reduction
to CO to 140 mV via stabilizing the CO2•- intermediate on the surfaces of the oxide-derived Au
electrodes.26 With respect to conversion, most studies focusing on electroreduction of CO2 to CO
report current densities in the range of 2 to 118 mA cm-2 under ambient condition, and most of
these studies use Ag as the cathode catalyst.14 For example, Dufek et al.59 and Delacourt et al.18 reported partial current densities for CO (jco) of less than 60 mAcm-2 at -1.8 V vs. Ag/AgCl when
operating their respective cells at ambient temperature and pressure. Tornow et al. studied nitrogen-based organometallic silver catalysts, which achieved jco as high as 115 mAcm-2 while
decreasing the Ag loading by a factor of 20.38 Also, recently we have reported that the performance
of Ag catalysts in CO2 reduction depends on Ag nanoparticle size.75
To date significant efforts have focused on the exploration of catalysts, whereas significantly fewer efforts have focused on the study of different catalyst supports. Catalyst supports can have tremendous influence on catalyst performance while simultaneously resulting in lower catalyst loading.76 For example, in fuel cells, reducing the loading of precious catalysts,
especially Pt, while increasing performance and durability, has been a critical step towards improving the commercial viability of this technology.76 Specifically, support materials have been developed to support and stabilize smaller nanoparticles that are often more active, while enabling better catalyst dispersion and utilization, and providing better electron conduction and mass transport.76-79
Titanium dioxide (TiO2) has been used as a readily available support material and a catalyst
for a variety of applications, including as a non-carbonaceous support for Pt in fuel cell electrodes80
and as a catalyst itself in the photo-reduction of CO2.81-84 TiO2 has been reported to interact
strongly with Pt, which increases the Pt catalyst activity, while at the same time increases the stability and durability of Pt catalysts.76,85,86 TiO2 can also act as a redox electron carrier to
facilitate various reduction reactions including CO2 conversion.87-89 Additionally, the TiO2 surface
has been reported to assist in CO2 adsorption90-93, thus it may be able to stabilize the CO2
•-intermediate to reduce the overpotential.
Here in this chapter, the use of TiO2 as a catalyst support for Ag catalysts to improve the
reduction of CO2 to CO will be reported. Previously, Cueto et al. observed enhancement of CO2
and/or H2O reduction when using Ag particles (~250 nm) that are electrodeposited on a thin film
TiO2 electrode.94 This work did not report product selectivity, and they did not study the role, if
any, of the flat TiO2 film. In contrast, the study reported here investigates the effect of much
smaller, sub-10 nm Ag nanoparticles deposited on 15-30 nm TiO2 particles on CO2
electroreduction. Specifically, two types of catalysts: different loadings of Ag catalyst supported on TiO2 (Ag/TiO2) and 40 wt% Ag supported on carbon black (Ag/C) were synthesized and
characterized. Their electrochemical performance in the reduction of CO2 to CO was compared
with the performance of the well-studied Ag nanoparticle catalysts using an electrochemical flow reactor.38,55 Through structural characterization and electrochemical experiments, the role of the TiO2 support in enhancing the catalytic sites, specifically with respect to its ability to maintain the
Ag nanoparticles at its most catalytically active size and its ability to stabilize the CO2
2.3.1 Preparation of Ag/TiO2 and Ag/C catalysts
The previously reported citrate-protecting method95,96 was used to obtain the different Ag/TiO2 catalysts. In contrast to previous reports, the support materials used here (TiO2 or carbon
black) were first mixed with 40 mM AgNO3 (Sigma-Aldrich) aqueous solution to allow for better
adsorption of Ag+ on the support. Sodium citrate (Fisher Chemicals) was then added to stabilize Ag+ followed by the addition of NaBH
4 (Sigma-Aldrich) to reduce Ag+. Specifically, for the
synthesis of 40 wt% Ag/TiO2, AgNO3 (125.7 mg) was dissolved in Millipore H2O (18.5 mL), TiO2
(120 mg, Aeroxide® TiO2 P25, particle size: 21±5 nm) was added to the solution, followed by
stirring for 30 minutes. Subsequently, sodium citrate solution (131 mM, 18.5 mL) was added drop by drop while stirring. The reduction of Ag+ was achieved by the drop-wise addition of NaBH4
solution (30 mM, 25 mL) with vigorous stirring in an ice-bath. After stirring the solution gently overnight, it was centrifuged, washed and dried in a vacuum oven at 80 °C for 4 hours. The obtained catalyst was wine red in color. Samples with Ag loadings of 5 wt%, 10 wt%, 20 wt%, and 60 wt% were prepared using the same method by changing the amount of TiO2. For
comparison, 40 wt% Ag/C catalyst was synthesized with the same method using Vulcan XC-72R (Carbon Blk Vulcan XC-72R, Fuel Cell Store) as the support.
2.3.2 Physical characterization
The Ag weight percentages of the different catalysts were determined by ICP-OES (PerkinElmer – Optima 2000DV). The samples were digested in a mixture of HNO3 and HF prior
to analysis. Ag particle size and dispersion on the support were examined using TEM (JOEL 2100 CRYO) operated at 200 kV. The TEM sample was prepared by suspending the catalyst in
isopropanol and placing a drop of the suspension onto a holey carbon-coated 200 mesh grid followed by solvent evaporation overnight at room temperature.
2.3.3 Electrochemical characterizations
Electrode preparation: Catalyst inks were prepared by mixing Millipore water (200 μL),
catalyst (2 mg), Nafion® solution (2.6 μL, 5 wt%, Fuel Cell Earth), and isopropyl alcohol (200 μL). The inks were then sonicated (Vibra-Cell ultrasonic processor, Sonics & Materials) for 15 minutes and then painted on the microporous layer of Sigracet 35 BC gas diffusion layers (Ion Power) using a paintbrush. All the flow reactor experiments in this study used a 1 mg cm-2 cathode catalyst loading on Sigracet 35BC, while all of the anodes used in this study had a 1 mg cm-2 Pt loading on Sigracet 35BC.
Electrochemical flow reactor operation: The flow reactor (see Supporting Information
Figure 2.6 for a schematic) was operated under ambient condition. A potentiostat (Autolab
PGSTAT-30, EcoChemie) operating in steady-state chrono-amperometric mode was used to measure the resulting current as previously reported.38 For each trial, five cell potential from -2.0 V to -3.0 V, with an interval of 0.25 V was applied to the cell. For each potential, the cell was allowed to reach steady state for 200 s, after which, the gas flowed into a gas chromatograph. The current was averaged for an additional 180 s before stepping to the next potential. The individual electrode potentials were measured using multimeters (AMPROBE 15XP-B) connected to each electrode and a Ag/AgCl reference electrode (RE-5B, BASi) placed in the exit stream. A mass ﬂow controller (MASS-FLO®, MKS instrument) was used to ﬂow CO
2 from a cylinder at 7 SCCM.
A syringe pump (PHD 2000, Harvard Apparatus) supplied the 1 M KOH electrolyte at 0.5 mL min-1. Gas products formed on the GDE surface and left through the GDE to the gas stream driven